| ||Format||Pages||Price|| |
|41||$71.00||  ADD TO CART|
|Hardcopy (shipping and handling)||41||$71.00||  ADD TO CART|
|Standard + Redline PDF Bundle||82||$85.20||  ADD TO CART|
Significance and Use
5.1 Electronic circuits used in space, military, and nuclear power systems may be exposed to various levels of ionizing radiation. It is essential for the design and fabrication of such circuits that test methods be available that can determine the vulnerability or hardness (measure of nonvulnerability) of components to be used in such systems.
1.1 This guide presents background and guidelines for establishing an appropriate sequence of tests and data analysis procedures for determining the ionizing radiation (total dose) hardness of microelectronic devices for dose rates below 300 rd(SiO2)/s. These tests and analysis will be appropriate to assist in the determination of the ability of the devices under test to meet specific hardness requirements or to evaluate the parts for use in a range of radiation environments.
1.2 The methods and guidelines presented will be applicable to characterization, qualification, and lot acceptance of silicon-based MOS and bipolar discrete devices and integrated circuits. They will be appropriate for treatment of the effects of electron and photon irradiation.
1.5.1 Determination of the Need to Perform Device Characterization—For some cases it may be more appropriate to adopt some kind of worst case testing scheme that does not require device characterization. For other cases it may be most effective to determine the effect of dose-rate on the radiation sensitivity of a device. As necessary, the appropriate level of detail of such a characterization also must be determined.
1.5.2 Determination of an Effective Strategy for Minimizing the Effects of Irradiation Dose Rate on the Test Result—The results of radiation testing on some types of devices are relatively insensitive to the dose rate of the radiation applied in the test. In contrast, many MOS devices and some bipolar devices have a significant sensitivity to dose rate. Several different strategies for managing the dose rate sensitivity of test results will be discussed.
1.6 Low Dose Requirements—Hardness testing of MOS and bipolar microelectronic devices for the purpose of qualification or lot acceptance is not necessary when the required hardness is 100 rd(SiO2) or lower.
1.7 Sources—This guide will cover effects due to device testing using irradiation from photon sources, such as 60Co γ irradiators, 137Cs γ irradiators, and low energy (approximately 10 keV) X-ray sources. Other sources of test radiation such as linacs, Van de Graaff sources, Dymnamitrons, SEMs, and flash X-ray sources occasionally are used but are outside the scope of this guide.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E170 Terminology Relating to Radiation Measurements and Dosimetry
E666 Practice for Calculating Absorbed Dose From Gamma or X Radiation
E668 Practice for Application of Thermoluminescence-Dosimetry (TLD) Systems for Determining Absorbed Dose in Radiation-Hardness Testing of Electronic Devices
E1249 Practice for Minimizing Dosimetry Errors in Radiation Hardness Testing of Silicon Electronic Devices Using Co-60 Sources
E1250 Test Method for Application of Ionization Chambers to Assess the Low Energy Gamma Component of Cobalt-60 Irradiators Used in Radiation-Hardness Testing of Silicon Electronic Devices
F996 Test Method for Separating an Ionizing Radiation-Induced MOSFET Threshold Voltage Shift Into Components Due to Oxide Trapped Holes and Interface States Using the Subthreshold Current-Voltage Characteristics
F1467 Guide for Use of an X-Ray Tester (10 keV Photons) in Ionizing Radiation Effects Testing of Semiconductor Devices and Microcircuits
Military SpecificationsMIL-HDBK-814 Ionizing Dose and Neutron Hardness Assurance Guidelines for Microcircuits and Semiconductor Devices
ICS Number Code 31.080.01 (Semi-conductor devices in general)
UNSPSC Code 32111700(Semiconductor devices)
ASTM F1892-12, Standard Guide for Ionizing Radiation (Total Dose) Effects Testing of Semiconductor Devices, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top